A facile non-solvent induced phase separation process for preparation of highly porous polybenzimidazole separator for lithium metal battery application

The drawbacks of low porosity, inferior electrolyte wettability, low thermal dimensional stability and permissive lithium dendrite growth of the conventional microporous polyolefin-based separators hinder their widely application in the high power density and safe Lithium ion batteries. Herein, highly porous polybenzimidazole-based separator is prepared by a facile non-solvent induced phase separation process (NIPS) using water, ethanol, chloroform and ethyl acetate as the coagulation bath solvent, respectively. It was found that the ethanol is suitable to fabricate uniform morphology macroporous separator with the porosity of 92%, electrolyte uptake of 594 wt.%, and strong mechanical strength of 15.9 MPa. In addition, the experimental tests (electrochemical analysis and XPS test) and density functional theory calculation suggest that the electron-rich imidazole ring of polybenzimidazle can enhance Li+ mobility electrostatic attraction interaction while the block the PF6− mobility via electrostatic repulsion interaction. Therefore, high Li+ transference number of 0.76 was obtained for the neat polybenzimidazole-based polymer electrolyte. As a proof of concept, the Li/LiFePO4 cell with the polybenzimidazole-based polymer electrolyte/1.0 M LiPF6− ethylene carbonate/dimethyl carbonate (v:v = 1:1) electrolyte exhibits excellent rate capability of >100 mAh g−1 at 6 C (1 C = 170 mA g−1) and superior cycle stability of 1000 cycles.

www.nature.com/scientificreports www.nature.com/scientificreports/ conductivity [22][23][24] . Moreover, the polyolefin based separators have poor compatibility with the electrolyte due to its hydrophobicity, which hampered fast absorption of large amount of electrolytes for effective ionic mobility 25 .
As one of the most popular engineering plastics, the fully aromatic polybenzimidazole (PBI) has intrinsically high thermal stability (thermal decomposition, T d > 550 °C). Li et al. fabricated the porous PBI-based separator via water vapor induced phase immersion method, the as-prepared membrane possesses the porosity of 81%, and electrolyte uptake of 328% 26 . Liang and his co-workers performed a blending phase inversion to prepare the micropores of PBI-based membrane via extracting poly(ethylene glycol)−10000 (PEG-10000) from the dry OPBI/PEG blend membranes with water 27 . The high porosity of 70% and electrolyte uptake of 316% were achieved when the PEG-10000 content was up to 150 wt.%. However, the mechanical property was largely sacrificed and the mechanical strength was decreased to 10 MPa, which is about two-thirds of commercial Celgard 2400 separator.
The lithium ion transference number ( + t Li ) is one of the most critical parameters of the electrolyte for application in lithium metal batteries by suppressing lithium dendrite growth. The relationship between the + t Li and lithium dendrite growth can be illustrated by using the Equation: τ = π − ( ) D eC Jt 2 0 , where τ is time consume to achieve complete ion depletion, D is the ambipolar diffusion coefficient, e is the electric charge, C 0 is the initial concentration, J is the current density and tis the transference number of anions. It indicates that reduce the t − or increase transference of + t Li can increase the deplete time of Li + and suppress lithium dendrite growth. In the present, a facile non-solvent induced phase separation process was performed to fabricate highly porous PBI-based membranes by using four different non-solvent, water, ethanol, chloroform and ethyl acetate as the coagulation bath solvent, respectively (Fig. 1b). The results indicate that ethanol induced phase separated porous membrane possesses highest porosity of 92% and electrolyte uptake of 594%, which are almost 3 times and 7 times higher than those of commercial PP separator, respectively. In addition, the porous membrane displays a strong mechanical strength of 15.8 MPa, which is even higher than the value of 14.5 MPa for commercial PP separator. It is beneficial for both incorporation of more electrolytes and uniform Li stripping/plating 28,29 . In addition, the strong electron-rich feature of imidazole ring favors Li + dissociation from lithium salt by the strong conjugated interaction (Fig. 1c), enhances Li + diffusion and hence its transference number. The Li + transference number of PBI-based polymer electrolytes without any additives is as high as 0.76 30 . After impregnation of 1.0 M LiPF 6 − EC/DMC (v:v = 1:1) into the p-PBIPE membrane, the Li/LiFePO 4 cell (Fig. 1d) exhibits excellent rate capability and superior cycle stability for over 1000 cycles at 6 C. These make the PBI-based polymer electrolyte for advanced Li metal batteries with high safety and performance.

Results and Discussion
Membrane morphology. To prepare a polymer electrolyte membrane with high porosity and appropriate mechanical strength, four solvents (water, ethanol, ethyl acetate and chloroform) are selected as the coagulation bath for the NIPS process, where the as-prepared membranes are denoted as wp-PBIPE, ep-PBIPE, ap-PBIPE, www.nature.com/scientificreports www.nature.com/scientificreports/ and cp-PBIPE, respectively. Scanning electron microscopy (SEM) images of the four membranes are shown in Fig. 2, and the key parameters, such as porosity, electrolyte uptake and mechanical strength, are listed in Table 1. The wp-PBIPE ( Fig. 2a and a') and ep-PBIPE ( Fig. 2b and b') membranes display more favorable pore architectures than that of the ap-PBIPE (Fig. 2c and c') and cp-PBIPE ( Fig. 2d and d') membranes. Simultaneously, the wp-PBIPE and ep-PBIPE show much higher porosities and more electrolyte uptake than those of the ap-PBIPE and cp-PBIPE ( Table 1). The ap-PBIPE exhibits the highest mechanical strength of 23.5 MPa, while the high toxicity as well as high cost of the ethyl acetate hinders its large-scale application. In addition, the non-uniform pore architecture gives rise to detrimental effect on the battery performances 31 . In particular, the ep-PBIPE exhibits high porosity and appropriate mechanical strength of 15.9 MPa, higher than mechanical strength of 14.5 MPa in the transverse direction for the commercial Celgard separator 32,33 , which is greatly beneficial for improving battery cycle stability 34,35 . Furthermore, the ep-PBIPE displays uniform and interconnected pore structure, indicating the smooth Li + diffusion, which is similar to the commercial Celgard separator (Fig. S1). Besides, the low cost and low toxicity of the ethanol coagulation bath makes the ep-PBIPE promising for large-scale application. conjugated interaction. The strong interaction between Li + and electron-rich imidazole ring to promote Li + diffusion are proved by X-ray photoelectron spectroscopy (XPS) and density functional theory (DFT) calculations. As depicted in Fig. 3a, two peaks are observed at around 398.7 eV and 397.1 eV for the neat PBI membrane, corresponding to the -N = (sp 2 hybrid N atom) and -NH-(sp 3 hybrid N atom) of the imidazole ring, respectively. However, one peak disappears after immersing the PBI membrane into 1.0 M LiPF 6 in EC/DMC (v:v = 1:1) electrolyte and another peak shifts to 400.3 eV, indicating that the strong interaction forms between LiPF 6 and PBI backbone.
As illustrated in Fig. 3b and Table S1, DFT calculations indicate that the highest occupied molecular orbital (HOMO) of the electron-rich imidazole ring in PBI can matches well with the lowest unoccupied molecular orbital (LUMO) of the Li + in LiPF 6 to form N-Li conjugated bond with the bonding distance of 1.988 Å and bonding energy of −49.194 kcal mol −1 . By contrast, the electron-rich imidazole ring shows repulsive interaction to PF 6 with long bonding distance of 3.415 Å and bonding energy of 4.741 kcal mol −1 (Figs. 3c and S2). The formed conjugated bond contributes to the Li + dissociation from PF 6 − , serving as another Li + pathway in ep-PBIPE membrane while the movement of PF 6 − is restricted (Fig. 3d).
Li + transference number, Li stripping/plating performance and morphology of Li metal anode.
The Li ion transference number of ep-PBIPE/LiPF 6 was measured by a steady-state current method on the Li|electrolyte|Li symmetric cell asseblied with the ep-PBIPE/LiPF 6 and PP-LiPF 6 − EC/DMC electrolyte at room temperature, the impedance spectra and the time-dependence response upon DC polarization are displayed in Fig. 4a. It shows that the Li ion transference number of ep-PBIPE/LiPF 6 electrolyte consequently increases from 0.23 (Fig. S3) for the Celgard/LiPF 6 electrolyte up to 0.76, which is beneficial to improve the stability of Li stripping/plating, in particular, to suppress lithium dendrite growth 36    www.nature.com/scientificreports www.nature.com/scientificreports/ is depicted in Fig. 4b. It depicts that the resistance becomes constant after 4 day, demonstrating a stable interface between the Li and ep-PBIPE.
The stripping/plating performance of metallic lithium anodes was determined by the galvanostatic Li stripping/plating cycling test and the results are shown in Fig. 4c. Li/Li symmetric cell at 0.5 mA cm −2 with the ep-PBIPE/LiPF 6 electrolyte exhibits a stable voltage profile, which is consistant with the previously reported anion-anchoring single ion conducting polymer electrolytes [37][38][39] . In contrast, Li/Li symmetric cell with the Celgard/LiPF 6 electrolyte shows fluctuating voltage profile with increasing voltage hysteresis, stemming from the depletion of cations at the Li/electrolyte interface 40,41 . Figure 4d-f shows the SEM images of Li foil with ep-PBIPE/ LiPF 6 electrolyte and Celgard/LiPF 6 electrolyte after long cycles of stripping/plating. The top surface of Li electrode with ep-PBIPE/LiPF 6 electrolyte is relatively uniform (Fig. 4d), without an overgrowth of dendrites, which is similar with the neat Li foil (Fig. 4e). In contrast, the Li foil in Celgard/LiPF 6 electrolyte exhibits a mossy, dendritic deposition (Fig. 4f).
Thermal stability and fire-retardancy. It is known that good thermal stabilities, including high thermal decomposition temperature and good dimensional stability are key parameters for battery separators, playing a vital role in preventing the thermal runaway when commercial batteries overheat caused by overcharge, overdischarge, internal and external short circuit or accidents [42][43][44] . Thermo-gravimetric (TG) analysis is employed to investigate the thermal stability of the Celgard separator and ep-PBIPE. As shown in Fig. 5a, the thermal decomposition temperatures reach up to 400 °C and 550 °C, respectively, for the Celgard separator and ep-PBIPE, which are much higher than the required temperature of 80 °C. However, differential scanning calorimeter (DSC) analysis in Fig. 5b reveals that the Celgard separator possesses soften point and melting point at 132 °C and 157 °C, respectively, representing the poor thermal dimensional stability (Fig. 5c). In contrast, no endothermic peak is observed for the ep-PBIPE even at high temperature of 350 °C, which is consistent with the high thermal dimensional stability without any shrinkage at 300 °C. Moreover, the fire-retardancy tests indicate that the ep-PBIPE is nonflammable and exhibit intriguing fire-retarding properties, benefiting from the intrinsic flame-retardancy of PBI (Fig. 5d-g).

Wettability
. Figure 6a-f shows the electrolyte wettability of the Celgard separator and ep-PBIPE determined by the contact angle measurements. The Celgard separator displays a slow electrolyte wetting with high contact angle of 51° after 90 s (Fig. 6a-c). The poor electrolyte wetting is caused by the nonpolar nature of the polyolefin polymer, originated from an intrinsically hydrophobic property and low surface energy 45,46 . In contrast, the electrolyte completely penetrates into the ep-PBIPE within 10 s (Fig. 6d-f). Besides the rather different pore structures, the fast electrolyte wetting of the ep-PBIPE is attributed to its highly polar imidazole ring. Accordingly, the superior electrolyte wetting leads to good electrolyte interfacial contact and small interfacial resistance 26,47 . electrochemical performance. The high ionic conductivity and good electrode compatibility of polymer electrolytes are crucial for the power density of LIBs. The temperature dependence of ionic conductivity of . Even at high current density of 6C, it still maintains high discharge capacity of >100 mAh g −1 (Fig. 7d), which is much higher than that of 87 mAh g −1 for the cell with Celgard separator. The cycling performances with two electrolytes at 6C are shown in Fig. 7e. The Li/LiFePO 4 cell with the ep-PBIPE-based electrolyte delivers an initial discharge capacity of 101 mAh g −1 , higher than that of 83 mAh g −1 for the Celgard-based electrolyte, and the capacity retention is 92.1% after 1000 cycles, corresponding to a  www.nature.com/scientificreports www.nature.com/scientificreports/ capacity loss of 0.0079% per cycle, which is attributed to excellent electrochemical stability (Fig. S4). Furthermore, we found that the coulombic efficiency of ep-PBIPE-based separator is much lower than that of Celgard separator after ~600 cycles. As we know that when the coulombic efficiency reaches below 95%, it suggests the failure of the lithium metal battery. Therefore, the stable cycling might be achieved by overwhelm usage of lithium metal rather than the merits of the separator. These results suggest that the ep-PBIPE membrane exhibits high potential application in high-density and safe Li metal batteries.
In conclusion, a series of PBI-based polymer electrolytes (p-PBIPEs) were successfully fabricated via a facile non-solvent induced phase separation process. The results indicate that ethanol is the best coagulation bath for highly porous p-PBIPE (ep-PBIPE) membrane with well-interconnected sponge-like pore structure and appropriate mechanical strength. In particular, the strong conjugated interaction between Li + and electron-rich imidazole ring is greatly favorable for improving the Li + dissociation and migration, subsequently increasing Li + transference number up to 0.76, and can effectively suppress the lithium dendrites growth. This enables stable Li stripping/plating for more than 400 h. In addition, the highly rigid and fully aromatic PBI backbone results in high thermal stability of ep-PBIPE membrane even at 300 °C, and the high polarity of imidazole ring and high porosity guarantees fast electrolyte wetting within 10 s. The Li/LiFePO 4 battery with the ep-PBIPE membrane exhibits excellent rate performance of >100 mAh g −1 at 6C and outstanding electrochemical stability for 1000 cycles.

Experimental Section
Materials. Polybenzimidazoles (PBI) was purchased from Suzhou Pinyu Optoelectronics Technology Co., Ltd. Lithium iron phosphate (LiFePO4), PVDF, and conductive agent (Acetylene Black) were purchased from Shanghai Darui Fine Chemical Co., Ltd., and used as received. N,Ndimethylacetamide (DMAC, AR, Aladdin) www.nature.com/scientificreports www.nature.com/scientificreports/ and N-Methyl-2-pyrrolidone (NMP, Anhydrous grade, 99.5%, Aladdin) were used as received. PP membrane (Celgard 2400) was cut into 19 mm film for use. fabrication of p-pBipe membranes. The non-solvent induced phase separation process was conducted according to our previous publication 45 . To investigate the effect of different coagulation bath solvents on the properties of the membranes, the four solvents with different polarity, water, ethanol, ethyl acetate and chloroform, were selected as solvents. As illustrated in Fig. 8, the calculated amount of PBI was first dissolved in N, N-dimethylacetamide (DMAc) to prepare a 12.5 wt% uniform casting solution. Afterward, the homogenous solution was cast onto a clean glass plate to prepare a film with average thickness of 35 µm. The film was quickly immersed in the mentioned four coagulation baths for 0.5 h to exchange DMAc solvent. Finally, the formed p-PBIPEs were dried at room temperature for 12 h followed by at 100 °C for 24 h in a vacuum oven.
preparation of Lifepo 4 electrode and battery assembly. The LiFePO 4 cathode consisting of a mixture of LiFePO 4 active material, acetylene black (AB) and binder of PVDF at a mass ratio of 7:2:1 was prepared by the following steps. PVDF binder was firstly dissolved in NMP, and the well-mixed mixture was then added into the above solution and stirred for at least 4 h to form homogeneous slurry. After that, the slurry was cast on an aluminum foil, dried at 60 °C for 12 h, and cut into 15 mm discs for use as the cathode of a coin cell and the mass loading of the cathode is approximately 4 mg cm −2 . Finally, the as-prepared cathode film was completely dried at 80 °C in a vacuum oven overnight and then transferred into an argon-filled glove box for further characterization. The Li/LiFePO 4 half-cells were assembled with p-PBIPE membrane and Celgard as separators and 1.0 M LiPF 6 − EC/DMC (v/v = 1:1) as electrolyte.
characterization. The morphology of the membranes was studied using a scanning electron microscope (FE-SEM, SU8010, HITACHI). Samples must be sprayed with gold for 100 s before testing. The interaction between p-PBIPEs membrane and LiFP 6 was analyzed by the X-ray photoelectron spectroscopy (XPS, Escalab 250xi, Thermo Fisher) and the testing samples were the p-PBIPEs membranes before and after immersed in 1 M LiPF 6 /EC/DMC (v:v = 1:1). The tensile strength and elongation tests of membranes were indicated using a tensile tester XLW (PC) at a strain rate of 25 mm/min. The thermal stability of membranes was characterized thermogravimetric analyzer (STA 449 F3, Germany NETZSCH) under an atmosphere of nitrogen with temperature range of from 30 to 800 °C at a rate of 10 °C min −1 . The endothermic and exothermic behaviors were investigated using Differential Scanning Calorimetry (METTLER TOLEDO DSC3) under nitrogen flow from 30 to 350 °C. The wettability of membranes with electrolyte was conducted by static contact angle and electrolyte spreading test. The thermal shrinkage test was performed by putting the membranes in a heating plate at various temperatures (150, 200, 250 and 300 °C), for 0.5 h at each temperature. The electrochemical stability was measured by the cyclic voltammetry (CV) with the membrane was sandwiched by a lithium electrode and a stainless steel (SS) electrode. The voltage was swept at the scan rate of 0.5 mV s −1 from −1.0 V to 5.0 V (vs. Li/Li + ).
The electrolyte uptake of the membrane was measured by immersing the membrane in a liquid electrolyte (1 M LiPF 6 in EC / DMC, 1:1 v/v) for 24 h for achieving complete soakage. The weights of dry membrane (M 0 ) and wet membrane (M 1 ) were obtained by accurately weighing the mass before and after the membrane soakage. The electrolyte uptake was calculated by the following Eq. (1): The process for determination of porosity (P) of the membrane is as follows. The dry membrane was immersed in n-butanol for 24 h for soaking the solvent in pore. The weight of the dry membrane and wet membrane were measured, respectively, and then the porosity was calculated according to the following Eq. (2): www.nature.com/scientificreports www.nature.com/scientificreports/ where W d is the dry weight of membrane, W w is the wet weight of membrane, ρ b is the density of n-butanol and V m is the volume of the membrane.
The ionic conductivity (σ) of polymer electrolytes was tested using electrochemical impedance spectroscopy (EIS) by sandwiching the electrolyte-soaked membrane between two stainless steel (SS) electrodes. The impedance data was recorded over a frequency range from 10 6 Hz to 1 Hz and the oscillating voltage of 5 mV. The ionic conductivity (σ) was calculated by the following Eq. (3): where l and A are the thickness and effective area of a membrane, respectively. And R is the impedance (Ω) of the membrane measured by EIS. The lithium ion transference number (t + ) was measured by sandwiching the membrane between two lithium electrodes. The lithium ion transference number (t + ) was calculated by the following Eq. (4): where ΔV is the set polarization voltage, I 0 and I S are the initial and steady-state currents, and R 0 and R S are the initial and steady-state resistances of the passivating layers on the Li electrode.